In the previous discussion of polaron effects in nitride QDs, the inﬂuence of the larger polar coupling and intrinsic electrostatic ﬁelds was studied using an effective-mass approach.

Effects originating from the wurtzite crystal structure and strong band-mixing have been considered neither in the QD wave functions nor in the energy dispersion of WL carriers.

The inclusion of such effects within an empirical tight-binding (TB) approach is subject to this chapter.

In the following, the basic idea of the empirical TB approach is presented, as well as a pro-cedure to incorporate the corresponding results in a many-body theory. For the description of QD properties, the inclusion of the WL plays a crucial role [146, 168]. Therefore, some comments on the inclusion of the WL in our calculations are in order. As discussed below, the localized QD wave functions are calculated in a ﬁnite supercell. Were we to directly model the combined QD-WL system within a supercell, we would have to use periodic boundary conditions that could lead to numerical artifacts due to coupling between the QDs in different instances of the supercell. Moreover, such a procedure would imply an unrealistic periodic array of QDs. Therefore, we include the WL along similar lines as dis-cussed Chap. A.1 using the envelope function-approximation. In a ﬁrst step, independent calculations for QD and QW states are performed and in a second step the OPW orthog-onalization procedure is applied for the combined QD-WL system. This approach on the one hand has the advantage of reducing numerical complexity and on the other hand ac-counts for the random distribution of QDs of the WL plane. Incorporating the random QD distribution is of central importance, as in this case the in-plane momentum is conserved on average (cf. Chap. A.1).

The results presented in the following have been obtained in close collaboration with Michael Lorke and Stefan Schulz. Stefan Schulz provided the TB wavefunctions and the dipole interaction matrix elements, whereas the calculation of Coulomb interaction matrix elements, polaron renormalizations, and absorption spectra was performed together with Michael Lorke.

**7.2.1 Empirical tight-binding model for bulk semiconductors**

The basic assumption of the TB approach is that electrons are tightly bound to their ions.

Therefore one chooses as basis states the eigenfunctions to the atomic problem, which are
the atomic orbitals. Correspondingly, the Schrödinger equation for an electron in a crystal,
[H^{atom}+ ΔV(R)] ψ(r) =E ψ(r), (7.4)
is separated into the atomic problem and the Coulomb potential originating from all other
electrons. The wavefunction for the solid then can be expanded in terms of atomic orbitals

φ** _{R,σ}** localized at the various lattice sites

**R**, ψ(r) =

**R,σ**

c_{σ}(R)φ** _{R,σ}**(r). (7.5)

The indexσ ∈ {α, ν, s}denotes the atomic orbital typeα(e.g. sp^{3} basis), the atom type
νand the spins. In case of bulk semiconductors, Bloch’s theorem might be employed due
to translational invariance and from an expansion into plane waves we ﬁnd

|k=
V_{0}

V

α,ν,s

**R**

e^{ikR}c_{α,ν,σ}(k)|R, α, ν, σ. (7.6)

Here, the spatial dependence of the TB coefﬁcientsc_{σ}(R)is reduced to a single unit-cell
by means of Bloch’s theorem. Using this expansion then yields a Schrödinger equation for
the TB coefﬁcients,

**R**^{},σ^{}

σ,**R|**Hˆ^{TB}|σ^{},**R**^{} c^{α}_{σ}_{}(R^{}) =E^{α}c^{α}_{σ}(R). (7.7)

The atomic orbitals from different lattice sites are in general not orthogonal. In this situa-tion a transformasitua-tion to orthogonalized Löwdin orbitals can be employed, which preserves the localization and symmetry properties of the atomic orbitals [33].

In Eq. 7.7, the dominant contributions arise from nearest-neighbor coupling because of the strong localization of the atomic orbitals. One observes that for bulk semiconductors the TB matrix can be reduced to a small number of TB parameters. A detailed evaluation of the TB overlaps is beyond the scope of this introduction and can be found for example in Ref. [33]. Thus, from a physical point of view the TB approach is quite intuitive, as the wave function is basically determined from the overlap of neighboring atomic orbitals.

Extensions of the basic TB model include spin-orbit coupling, crystal-ﬁeld splitting, intrin-sic piezoelectric ﬁelds, and strain ﬁelds. Technical details can be found in Ref. [33]. For nitride semiconductors, especially the inclusion of spontaneous and strain-induced electric ﬁelds is of central importance [193]. The spontaneous polarization for various alloys is known from the literature [179]. On the other hand, the inclusion of the strain-induced part of the piezo-electric polarization is more involved. In this case the strain ﬁeld for the particular situation, elastic moduli, and piezoelectric constants have to be considered [194].

The corresponding electrostatic potential is obtained from the solution of Poisson’s
equa-tion. Within the TB model the resulting electrostatic ﬁelds can be included as site-diagonal
contributionsV_{p}(r) =−eφ_{p}(r)to the Hamiltonian. This approach is also successfully
ap-plied to QW [195] and QD [196] structures.

**7.2.2 The QD model**

For the calculation of QD wave functions within the TB approach, the utilization of Bloch’s theorem is not possible due to the lack of translational invariance. Instead, a ﬁnite supercell with zero boundary conditions is introduced. Such a supercell including a lens-shaped QD is schematically shown in Fig. 7.6. Additionally the corresponding spatial dimensions are given. The particular QD that we consider in the following consists of pure InN and is located on top of an InN WL, grown in the (0001)-direction. QD and WL are embedded in a GaN matrix.

00 00 00 00 00 00 00 00 00 00 00 00 00 00 00 00 00 00 00 00 00 0

11 11 11 11 11 11 11 11 11 11 11 11 11 11 11 11 11 11 11 11 11 1

1.6 nm 4.5 nm

**InN WL**
**InN QD**

**GaN**

18.5 nm

7.0 nm

16.0 nm

**Fig. 7.6: Super cell and QD geometry for the calculation of QD states. Picture courtesy of**
Stefan Schulz, [33].

The QD wave functions are calculated from a numerical diagonalization of the TB
Schrö-dinger equation (7.7). As an approximation, the corresponding TB parameters known
from bulk semiconductors are used σ,**R|**H|σ^{},**R**^{} ≈ σ,**R|**H^{bulk}|σ^{},**R**^{}. For the TB
matrix, at each lattice site of the supercell the corresponding TB parameters are chosen
according to the species of the occupying atom (In, Ga or N). At the InN/GaN interfaces
of the nanostructure the assignment of the N atoms is ambiguous. In this case an averaging
between InN and GaN parameters is employed [33, 197]. The the band gap of GaN and
InN as well as the band offsets for valence and conduction band are chosen according to
recommendations in the literature [32, 179]. For the valence band, an offset of 0.5 eV is
included as a energy shift in the site-diagonal TB matrix elements for the bulk material
[32]. Additionally, also the intrinsic electrostatic ﬁelds are considered as site-diagonal
energy shifts. Spin-orbit coupling and crystal-ﬁeld splitting is neglected, as they only give
rise to minor corrections. For a detailed investigation see Ref. [33, 197].

**s : 0.754**
p_{x}: 0.051
p_{y}: 0.051
p_{z}: 0.144

**e****1**1.7320 eV

**s : 0.705**
p_{x}: 0.041
p_{y}: 0.136
p_{z}: 0.118

**e****2** 1.9621 eV

X Y

**s : 0.705**
p_{x}: 0.136
p_{y}: 0.041
p_{z}: 0.118

**e****3**1.9621 eV

s : 0.000
**p**_{x}**: 0.499**
**p**_{y}**: 0.499**
p_{z}: 0.001

**h**** _{1}**0.6256 eV

s : 0.006
p_{x}: 0.144
**p**_{y}**: 0.834**
p_{z}: 0.016

**h**** _{2}** 0.6158 eV

s : 0.006
**p**_{x}**: 0.834**
p_{y}: 0.144
p_{z}: 0.016

**h**** _{3}** 0.6158 eV

**Fig. 7.7: Modulus squared of the QD wavefunctions in top view. The QD structure is**
depicted in gray whereas the iso-surfaces of the charge density are shown for 10% (blue)
and 50% (red) of the maximum value. Furthermore the orbital composition is given and
the dominant contribution is highlighted. Pictures courtesy of Stefan Schulz, [33, 157].

The TB wave functions were calculated by Stefan Schulz, [32, 33, 197, 198]. Fig. 7.7 shows results for the three energetically lowest conﬁned states of the QD geometry de-picted in Fig. 7.6. The ground state both for electrons and holes shows no degeneracy, apart from spin degeneracy. In contrast, the ﬁrst excited states are two-fold degenerate, which is due to the fact that spin-orbit coupling and crystal-ﬁeld splitting are not consid-ered. Including these contributions lifts the degeneracy [33, 197].

For the classiﬁcation of the electronic states some symmetry considerations are of para-mount importance. A detailed analysis in this respect is beyond the scope of the present thesis and we refer the reader to the excellent discussions in Refs. [33, 140]. Neverthe-less, we want to summarize the basic results of those considerations. In the following, a function that is invariant under discrete rotations around the z-axis is called “s-state”.

Correspondingly, if the state transforms like an atomic p-function under these rotations it
is called “p-state”. From the nodal structure of the wave functions shown in Fig. 7.7, a
classiﬁcation into s- and p-like states is directly evident for the electron states, but it is
much less obvious for the hole states. However, in fact such a classiﬁcation is possible
by analyzing the behavior of the hole states under symmetry operations of the underlying
group C_{3v}. The total symmetry of a wave function in TB representation is determined
by the symmetry of the atomic orbitals and that of the TB coefﬁcients. Comparing the
TB representation Eq. (7.5) with the envelope-function approximation Eq. A.1, we ﬁnd
that the atomic orbitals translate into the Bloch functions and the TB coefﬁcients are the
discretized analog to the envelope function. The weight of the different orbitals is given

in Fig. 7.7. As expected, we ﬁnd that the electron states are mainly composed of s-type
orbitals, while in the hole states mainly p-type orbitals contribute. Furthermore, we can
infer from the modulus of the wave functions shown in Fig. 7.7 that the symmetry of the
TB coefﬁcients is s-like for the ground state and p-like for the two excited states. These
symmetries of the orbital composition and the TB coefﬁcients in total result in an s-like
symmetry for the ground state and a p_{x}- and p_{y}-like symmetry of the two excited states,
both for electron and hole states.

**7.2.3 The WL model**

For the description of the combined QD-WL system we start from separate calculations for a QD and a QW, where in a second step the resulting QW states are orthogonalized to the QD states. The calculation of the localized QD states and their symmetry properties are discussed in the previous chapter. In this chapter corresponding calculation for a QW is presented, which additionally yields the energy dispersion of the delocalized WL states.

In contrast to the QD case, the TB calculation for a QW can be considerably simpliﬁed.

Due to translational invariance Bloch’s theorem can be employed in the WL plane and one
can restrict the calculation to a column of unit cells along the growth direction, as shown in
Fig. 7.8. Additional details on TB calculations for QW systems can be found for example
in Refs. [199, 200]. As the alert reader might notice, the application of Bloch’s theorem
in this system is not straightforward due to the existence of two layers within the unit cell
(cf. Figs. B.1 and 7.8). For convenience, we split **R** into an in-plane part and a z-part
according to

**R**= (R||+**f**l) +**R**z , (7.8)

where **R**|| is the in-plane position of the unit cell and**f**l denotes the in-plane position of
layerlwithin the unit cell. By this procedure we assure that**R**_{||}is always a lattice vector
and Bloch’s theorem for the double layer structure reads

c^{k}_{σ}(R) =c^{k}_{σ}(fl+**R**z) exp(i**kR**||). (7.9)
A further advantage of this approach is that a direct classiﬁcation of WL states using the
in-plane crystal momentumkis achieved. This is also desirable from a physical point of
view, as the in-plane translational invariance being present in the QW system, also holds
in the QD-WL system, at least on average.

For the diagonalization of the Schrödinger equation (7.7) for the TB coefﬁcients, again at each lattice site of the unit-cell column the bulk TB parameters according to the species of the occupying atom (In, Ga or N) are used and at the interfaces an averaging between InN and GaN parameters is employed. The calculation of the QW states has also been performed by Stefan Schulz. For the lowest conduction band (CB) and the two highest va-lence bands (VB), the resulting in-plane energy dispersion for the QW is shown in Fig. 7.9

wetting layer
*z = 0*

*x*
*z* layer 1 layer 2

**Fig. 7.8: Column of unit cells for the calculation of QW states, showing the double-layer**
structure of the wurtzite lattice.

Around theΓpoint, for the conduction band as well as for the two highest valence bands,
the dispersion is to a good approximation rotational invariant. For larger**k**ﬁrst the
hexag-onal structure of the real space lattice and later, rotated by 30°, the hexaghexag-onal structure of
the Brillouin zone is reﬂected in the energy dispersion. Furthermore, strong band-mixing
effects are observed, giving rise to the “oscillations” seen in the iso-surface lines.

Note, that due to the fact that the two highest VBs are energetically nearly degenerate
at theΓ-point, a restriction to only one VB, as we typically use it in the GaAs material
system is not applicable. Thus, for the calculation of optical properties we need to take
both VBs into account. For further calculations, we are only interested in the bandstructure
in the vicinity of theΓ-point. Therefore, in a good approximation we might use the
angle-averaged band structure, which is shown in Fig. 7.10. Even though the dispersion shows a
clear non-parabolic behavior, an estimate for the effective masses can be given from a ﬁt
in the vicinity of theΓ-point. For the CB we ﬁnd a mass of 0.18m_{0}, whereas for the upper
and lower VB -2.84m_{0} and -0.19m_{0}are found.

2 2.5 3 3.5 4 4.5 5 5.5 6

-15 -10 -5 0 5 10 15 kx in 1/nm

-15 -10 -5 0 5 10 15

ky in 1/nm

(a) CB

-2 -1.5 -1 -0.5 0 0.5 1

-15 -10 -5 0 5 10 15 kx in 1/nm

-15 -10 -5 0 5 10 15

ky in 1/nm

(b) lower VB

-2 -1.5 -1 -0.5 0 0.5 1

-15 -10 -5 0 5 10 15 kx in 1/nm

-15 -10 -5 0 5 10 15

ky in 1/nm

(c) upper VB

**Fig. 7.9: Energy dispersion as a function of the 2D in-plane wavevectork**for the
conduc-tion and valence band. The hexagonally shaped border of the Brillouin zone is marked in
black.

0 0.5 1 1.5 2 2.5 3 3.5

0 0.5 1 1.5 2 2.5

energy in eV

k in 1/nm 0.56 0.58 0.6 0.62 0.64

0 0.5 1

energy in eV

k in 1/nm

**Fig. 7.10: Angle-averaged in-plane energy dispersion. The dots mark the energies of the**
QD states obtained from their respective TB calculation.

**7.2.4 Evaluation of Coulomb matrix elements**

An atomistic approach like a tight-binding calculation allows to account for symmetry
properties of the wurtzite crystal structure. The wavefunction is expressed as a linear
combination of atomic orbitalsφ** _{R,σ}**localized at the lattice site

**R**,

ψ(r) =

**R,σ**

c_{σ}(R)φ** _{R,σ}**(r), (7.10)

with the index σ denoting the orbital types (sp^{3} basis) at each lattice site. For the
calcu-lation of single-particle energies, the explicit knowledge of the localized orbital functions
is not needed within a TB approach. To calculate Coulomb matrix elements, in principle
they are required. However, the dominant contributions to the Coulomb matrix elements
stem from its long-ranged part and therefore the localized orbitals in good approximation
act as point charges. The explicit structure of the localized orbitals enters only in the
short-ranged contributions. Therefore, the real space integration of wavefunctions in Eq. (4.1)
might be approximated by a sum over TB coefﬁcients at their lattice sites,

V_{αβγδ}≈ e^{2}
4πε_{0}ε_{B}

**RR**^{}

στ

c^{α∗}_{σ} (R)c^{β∗}_{τ} (R^{}) 1

|R−**R**^{}| c^{γ}_{τ}(R^{})c^{δ}_{σ}(R). (7.11)

This scheme can be easily used when the analysis is restricted to the localized states. It has been successfully used to determine Coulomb matrix elements for InN/GaN QDs in com-bination with conﬁguration-interaction (CI) calculations to describe multi-exciton spectra and the inﬂuence of symmetry properties on allowed optical transitions [33, 140, 157, 201]

For our purpose of calculating optical properties of nitride QDs, including both localized and delocalized states, it is more convenient to determine the Coulomb matrix elements from Eq. (4.1), involving the Fourier transform of the Coulomb potential. Using the same approximation for the real-space integration as above, the appearing overlap integrals can be written as

α|e^{iqr}|β =

d^{3}r ψ^{∗}_{α}(r)e^{+iqr} ψ_{β}(r) ≈

**R,σ**

c^{α∗}_{σ} (R)e^{+iqR}c^{β}_{σ}(R). (7.12)

As the plane waveexp(iqr)does not decay for large distances, the argument used to derive Eq. (7.11) also holds in this case. Note, that in Eq. 7.12 also the orthogonality of the atomic orbitals was used, giving rise to the fact that both coefﬁcients carry the same orbital index.

**Calculation of overlaps**

The overlaps for two QD states can easily be calculated using Eq. (7.12). Using Bloch’s theorem we also can evaluate the QD-WL overlaps directly

ν|e^{iqr}|k_{0} =

**R,σ**

c^{ν∗}_{σ} (R)e^{+iqR}c^{k}_{σ}(f +**R**z)e^{ikR}^{||} . (7.13)
Note, that for the numerical evaluation one eventually has to account for a different
nor-malization of the TB coefﬁcients for QD and QW states.^{1} The WL-WL overlaps require a
little more attention. However, we again can employ Bloch’s theorem and the fact, that the
unit cell has a double layer structure. This allows us to write

k0|e^{iqR}|k^{}_{0}= 1
N

σ,R

c^{∗}** _{k,σ}**(R) e

^{iqR}c

**,σ(R)**

_{k}= 1 N

2 l=1

**R**||

σRz

c^{∗}** _{k,σ}**(R) e

^{iq}

^{z}

^{R}^{z}e

^{iq}

^{||}

^{R}^{||}e

^{iq}

^{||}

^{f}^{l}c

**,σ(R)**

_{k}= 1 N

2 l=1

**R**_{||}

σRz

e^{iq}^{z}^{R}^{z} c^{∗}** _{k,σ}**(fl+

**R**z)c

**,σ(fl+**

_{k}**R**z)

e^{i(q}^{||}^{+k}^{}^{−k)R}^{||} e^{iq}^{||}^{f}^{l}

= 2

l=1

e^{iq}^{||}^{f}^{l}F_{l}(k,**k**^{}, q_{z}) 1
N

**R**||

e^{i(q}^{||}^{+k}^{}^{−k)R}^{||}

=δ_{q}_{||}_{,k−k}

2 l=1

e^{iq}^{||}^{f}^{l} F_{l}(k,**k**^{}, q_{z}).

(7.14) For the two layers of the unit celll = (1,2), separately a formfactor can be deﬁned,

F_{l}(k,**k**^{}, q_{z}) =

σRz

e^{iq}^{z}^{R}^{z}c^{∗}** _{k,σ}**(f

_{l}+

**R**z)c

**,σ(f**

_{k}_{l}+

**R**z).

Even though the deﬁnition of two separate formfactors is not necessary, it is of practical advantage as it allows to save computer memory. For the evaluation of the interaction ma-trix elements, the QW states|k0are then orthogonalized by means of the OPW procedure discussed in Chap. A.1.

1Usually in the QD calculation the TB coefﬁcients are normalized to the supercell and those of the QW
calculation are normalized to the unit-cell column. In wurtzite crystals one lattice point in the hexagon plane
is associated with the area ofS=a^{2}2

3/2, cf. the crystal structure in App. B.2.

**7.2.5 Dipole interaction matrix elements**

The dipole matrix elements for the QD-QD transitions can be directly obtained from the
TB calculation of the QD. Details on the calculation are presented in Refs. [33, 201] and
we summarize the numerical values in Tab. 7.1. For the particular QD geometry under
consideration we ﬁnd that direct transitions, i.e. s→s and p→p transitions, only weakly
couple to the electro-magnetic ﬁeld in comparison to the off-diagonal transitions s→p and
p→s. These selection rules deviate from the ones known for zincblende GaAs QD, where
one observes only direct transitions due to the Bloch functions. These “skew” selection
rules for nitride QDs are related to the underlying symmetry of the wurtzite lattice. As
e.g. for the ground-state transition the wave function for electrons as well as for holes
exhibits an s-like symmetry, the corresponding dipole transition is zero. In contrast, for
the GaAs the wave function in envelope function approximation obeys an s-like symmetry
for electrons and an p-like symmetry for holes, cf. Chap. A.3, yielding non-zero dipole
transitions. Whereas the ground-state transition exactly vanishes, the excited-state
transi-tions are non-zero but small due to the C_{6v} symmetry of the wurtzite lattice. In case of
an C_{∞v} symmetry, e.g. considered in**k**·**p**calculations, also the excited-state transitions
would vanish. For a detailed discussion of the symmetry properties we refer the reader to
Refs. [33, 140, 157].

d^{cv}/e 1 2 3

1 0.000 1.538 1.538 2 1.196 0.011 0.011 3 1.196 0.011 0.011

**Tab. 7.1: QD dipole matrix elements in nm from a TB approach with spontaneous and**
strain-induced electric ﬁelds included [33].

As in this thesis our focus is on QD transitions, a simpler treatment of the WL-WL dipole
matrix elements is affordable. We employ the results of a**k**·**p**model for a QW presented
in Ref. [181], utilizing the parameters recommended in Ref. [179]. However, for
com-pleteness a scheme for calculating the corresponding dipole matrix element from an TB
approach is outlined in App. A.3. Furthermore QD-WL matrix elements are neglected
for computational reasons, though they could be included along the lines discussed in
Ref. [33, 201] using Bloch’s theorem.